The Effect of Porcelain Firing and Type of Finish Line on the Marginal
Fit of Zirconia Copings
Mahroo Vojdani a, Anahita Safari b, Mina Mohaghegh b, Soheil Pardis c, Farideh Mahdavi d
Biomaterial Research Center, Dept. of Prosthodontics, School of Dentistry, Shiraz University of Medical Sciences, Shiraz, Iran.
b Dept. of Prosthodontics, School of Dentistry, Shiraz University of Medical Sciences, Shiraz, Iran. c
Dept. of Pathology, School of Dentistry, Shiraz University of Medical Sciences, Shiraz, Iran.
d Postgraduate Student of Prosthodontics, School of Dentistry, Shiraz University of Medical Sciences, Shiraz, Iran.
KEY WORDS Marginal fit;
Received April 2014;
Received in revised form May 2014; Accepted June 2014.
Statement of the Problem: Although all-ceramic restorations are broadly used, there is a lack of information concerning how their fit is affected by fabrication
pro-cedure and marginal configuration.
Purpose: The purpose of this study was to evaluate the marginal fit of zirconia CAD/CAM ceramic crowns before and after porcelain firing. The influence of finish
line configuration on the marginal fit was also evaluated.
Materials and Method: Twenty standardized zirconia CAD/CAM copings were fabricated for chamfer and shoulder finish line designs (n=10). The marginal fit of
specimens was measured on 18 points, marked on the master metal die by using a
digital microscope. After the crowns were finalized by porcelain veneering, the
measurements of marginal fit were performed again. The means and standard
devia-tions were calculated and data were analyzed using student’s t-test and paired t-test
Results: There were significant differences between marginal fit of chamfer and shoulder finish line groups before and after porcelain firing (p= 0.014 and p= 0.000,
respectively). The marginal gap of copings with shoulder finish line was significantly
smaller than those with chamfer configuration (p= 0.000), but there were no
signifi-cant differences between the two marginal designs, after porcelain firing (p= 0.341).
Conclusion: Porcelain veneering was found to have a statistically significant influence on the marginal fit of zirconia CAD/CAM crowns. Both margin configurations
showed marginal gaps that were within a reported clinically acceptable range of
Corresponding Author: MohagheghM., Postgraduate Student of Prosthodontics, School of Dentistry,
Shiraz University of Medical Sciences, Shiraz, Iran. Tel: +98-91737322950 Email: firstname.lastname@example.org
Cite this article as: Vojdani M., Safari A., Mohaghegh M., Pardis S., Mahdavi F. The Effect of Porcelain Firing and Type of Finish Line on the Marginal Fit of Zirconia Copings. J Dent
Shiraz Univ Med Sci., June 2015; 16(2): 113-120.
As far as esthetics and acceptable biocompatibility of
dental restoration are concerned, all-ceramic crowns
have recently gained large popularity. If made of high
quality, all-ceramic restorations are difficult to be
dis-tinguished from unrestored adjacent teeth. 
Among the many ceramic systems that have been
developed, [2-3] Yttria-stabilized polycrystalline
tetrag-onal zirconia has become a popular form of dental
resto-ration; mostly because of its notable characteristics
in-cluding esthetics, excellent biocompatibility, low plaque
accumulation, and high strength.  For the fabrication
of zirconium oxide core, computer-aided design/
com-puter-aided manufacturing (CAD/CAM) is used by the
system.  A compatible feldspathic translucent
white zirconia core to guarantee the excellent esthetics
of the restorations.  This veneering process which
includes a firing procedure (sintering) at high
tempera-ture (750-900°C) and subsequent cooling of the
restora-tion, is carried out at least once, but usually 2-5 times.
One of the most important standards in clinical
as-sessment and success of fixed dental restorations is
marginal fit of the crown. [7-10] In fact; marginal misfit
has many severe outcomes which may induce
prospec-tive failure of the prosthesis. Large marginal
dis-crepancies make the luting agent to be disclosed within
the oral environment. If the marginal gap is large, the
cement will decompose rapidly as a result of oral fluids
and chemomechanical forces.  This microleakage,
in part, results in secondary caries, pulpal inflammation,
and necrosis. [9-13] Inept marginal adaptation also
causes plaque retention and compositional changes in
the subgingival microflora, and consequently
inflamma-tion in gingival and periodontal tissues.  Finally,
marginal misfit generates stress concentrations which
may decrease the strength of the restoration. 
Marginal fit of the crown is defined as the gap
be-tween the prepared tooth and the intaglio surface of the
restoration. Absolute marginal discrepancy is the linear
distance between the cavosurface finish line of the
prep-aration and the margin of the restoration.  This
measurement displays the total misfit at the margin and
is always considered as the largest measurement of the
error at that point.  Mclean et al. defined clinically
acceptable marginal discrepancies to be between 40 to
120 µm.  Previous studies have reported marginal
discrepancy range of zirconia ceramic crowns to be 19
to 160 µm. [15, 19-23] However, there is limited studies
on the marginal fit of zirconia-based materials in
com-parison with conventional ceramic or metal restorations.
Given the importance of the fitting accuracy of
restoration,  there has been much debate on the effect
of veneering porcelain on all-ceramic restorations fit.
[15, 19-20, 25-27] To name a few, Balkaya et al.
report-ed that the porcelain firing cycle has an influence on the
marginal fit of In-ceram all-ceramic crowns. 
Cas-tellani et al. also pointed out that the marginal area of
single crowns manufactured with different all-ceramic
systems deforms significantly during the porcelain
ve-neering process.  Contrary to these findings, Pera et
al. found that the processes of firing and glazing of
vita-dur-N veneer did not alter the dimensional stability of
In-ceram substructures. 
Moreover, the effect of the type of marginal
de-sign on the fitting precision of restoration should also be
studied rigorously; for, there is no mutual agreement
concerning ideal margin configuration of all-ceramic
restorations. Researchers advocated either deep chamfer
or rounded shoulder finish lines. [20, 28] Some studies
on Procera ceramics  and zirconia ceramic crowns
 suggested a significant difference in marginal gap
between the two marginal designs. Based on their
find-ings, rounded shoulder was identified to perform better.
In contrast, some other studies illustrated that margin
configuration had no significant difference on the
mar-ginal fit of ceramic crowns. [20, 31-32]
Marginal discrepancy can, in fact, be measured by
using several methods such as direct view of the crown
on a die, cross-sectional view, impression replica
tech-nique, and clinical examination.  The direct view, as
used by the researchers of the current study, is a
non-destructive technique which is frequently employed to
measure the distortion during the manufacturing process
of the restorations. 
The purpose of this study was to evaluate the
marginal fit of zirconia CAD/CAM ceramic crowns
before and after porcelain firing. The influence of finish
line configuration on marginal fit was also evaluated.
The null hypothesis was that no differences would be
found in the marginal fit of zirconia CAD/CAM crowns
before and after porcelain firing, and among different
Materials and Method Fabrication of master dies
Brass master dies (Figure 1) were prepared for rounded
shoulder and deep chamfer margins in a lathe (CNC350;
Arix Co. Tainan Hesin, Taiwan).
Figure 2: Fabricated zirconia CAD/CAM copings
Preparation of master dies was done in accordance
with the current standards of full-ceramic restorations.
 The preparation was standardized using a 1 mm
wide smooth continuous margin, free of any
irregulari-ties, with occlusal convergence of 6 degrees with a
height of 7 mm. A ledge was formed at the
occluso-axial line angle to serve as anti-rotational feature. The
measuring areas for evaluation of absolute marginal gap
(AMG) were marked as 18 grooves at 20 degree
inter-vals with a high speed handpiece (KaVo K9; KaVo
dental GmbH, Biberach, Germany) and a diamond
nee-dle bur on a 2 mm groove below the margin. The
sam-ple size and the number of measurements per die were
selected based on previous published studies. [15-16]
Fabrication of the copings
The master dies were placed in a mold made of
baseplate wax and checked with a surveyor (Ney Dental
Surveyor; Dentsply, Ballaigues, Switzerland) to ensure
its parallelism. The master dies were maintained in their
place during acrylic packing by using wooden struts and
sticky wax. Next, the mold was filled with
auto-polymerized acrylic resin (DuraLay; Reliance Dental
Co., Place Worth, IL). In this manner, the groove below
the margin of the master die was 2 mm above the
acryl-ic surface. Impressions of master dies were made out of
additional putty and wash silicone materials (elite HD+;
Badia Polesine, Zhermack Rovigo, Italy) in special trays
(GC pattern resin; GC Corp., Tokyo, Japan). Twenty
working dies (n=10 per each group) were fabricated
using type IV dental stone (elite rock; Badia Polesine,
Zhermack Rovigo, Italy). The stone dies were visually
inspected for any possible irregularity by a single
opera-tor utilizing a binocular loupes (HEINE HR-C 2.5x;
HEINE, Herrsching, Germany). The stone dies were
coded and then scanned by a laser scanner (3Shape
D810; 3Shape, Copenhagen K, Denmark) for digitizing
the dies. The data were then transferred into a software
(3Shape's CAD Design software; 3Shape, Copenhagen
K, Denmark) in which the copings were designed with a
thickness of 0.5 mm considering the 30 µm spacer 1
mm short of margin.  Copings were machined out of
zirconium blanks (VITA In-ceram YZ-14; Vident,
Germany) which were made of partially stabilized
zir-conium powder mixed with a binder in a milling
ma-chine (CORiTEC 340i; Imes-icore GmbH, Eiterfeld,
Germany) (Figure 2). Before sintering, the copings were
steam cleaned. The machined copings, which had to be
25% larger than stone dies in order to compensate for
the sintering shrinkage, were transformed back into their
original size after the sintering. The copings were then
seated on the master dies.
Figure 3: Captured image of coping-die interface (Zirconia coping (A), Brass master die (B), marginal gap (C))
Marginal discrepancy evaluation
The process of marginal discrepancy evaluation started
with the copings being placed over the master dies using
a special metallic device. To measure the marginal fit of
the copings, the perpendicular measurement from the
internal surface of the restoration margin to the most
outer edge of the finish line of the preparation (AMG)
was taken at 18 previously- marked points by use of a
digital microscope (AM413FIT Lite Pro;
Dino-Lite electronic Corp., Taipei, Taiwan). The microscope
was mounted on a desktop stand (MS35B; Dino-Lite,
Taipei, Taiwan), connected to a personal computer (PC)
Figure 4: The completed crowns after porcelain firing
at 230 x magnification. High-resolution photographs
were captured and displayed on the computer monitor.
(Figure 3) Then, the measurements were taken based on
the produced images.
Porcelain firing cycles
At this stage, the copings were prepared for porcelain
application (Vita VM9; Vident, Germany). Porcelain
application was done 0.5 mm short of margin. [24, 33]
A silicone index was used to standardize the shape and
the size of veneers. Next, the dentin and enamel
porce-lain were applied. (Figure 4) After each step, porceporce-lain
thickness was measured with a gauge (POCO 2N;
Kroeplin, Schlüchtern, Germany). For all of the
cop-ings, porcelain application and firing cycles were done
by a skilled technician based on the current standards.
The marginal fit was measured again on the final master
dies at the previously marked points.
The means of different groups were compared using
student’s test at the significant level of 0.05. Paired
t-test was also performed to compare the amount of
mar-ginal fit before and after the veneering of porcelain
within the same group. (Figure 5)
Figure 5: Mean values of marginal gap before and after porce-lain firing
All statistical analyses were performed using SPSS 16.0
for windows (SPSS 16.00 for windows; SPSS Inc,
Table 1 shows the means and standard deviations for the
marginal gap of the specimens before and after
porce-lain firing in micrometers, sorted out by the margin
Table 1: Absolute marginal gap of zirconia copings and crowns (µm)
Copings Crowns P value Mean SD Mean SD
Chamfer 49.87 a 3.62 68.24 b 13.84 0.014 Shoulder 35.20 a 6.15 63.06 b 5.59 0.000
Different superscript letter in each row indicates
significant difference by student’s test at α=0.05.
There were significant differences between
mar-ginal fit of the two groups before and after porcelain
firing (p< 0.05). The mean score of marginal gap in
deep chamfer marginal design before and after the
porcelain application was 49.8 µm and 68.2 µm,
respec-tively. The mean score for marginal gap in rounded
shoulder marginal design was 35.2 µm before and 63.06
µm after the porcelain application. The marginal fit of
shoulder copings was significantly better than chamfer
copings (p= 0.000), but there were no significant
differ-ence between the two margins, after firing the porcelain
(p= 0.341). These findings suggest that porcelain firing
cycles change the marginal fit of shoulder copingsmore
adversely. For both margin configurations, the marginal
discrepancy of zirconia copings showed significantly
smaller gaps than that of completed crowns. However,
there was no significant difference between completed
crowns of both chamfer and shoulder marginal designs.
first part of the null hypothesis; since there was a
signif-icant difference in the marginal fit of zirconia
CAD/CAM crowns before and after porcelain firing.
However, no significant difference was observed
be-tween the two margin configurations of the finished
crowns. Thus, data support acceptance of this part of the
In the current investigation, the researchers used a
single metal die for each margin configuration. The
application of this single standard master die provided
standardized preparation and direct comparison of
mar-ginal discrepancies and also precluded any wear from
being formed during the manufacturing and measuring
processes. In addition, it prevented luting of individual
crowns onto the dies, an event which could affect the
marginal fit because of probable variance in luting
agent's viscosity and seating forces. 
Since porcelain contamination on the margin of
copings might influence the accuracy of measurements,
the application of porcelain was done 0.5 mm short of
margin. In addition, this procedure finely restrained
partial seating of the crowns which could occur as a
result of intaglio surface contamination. [24, 34]
The obtained mean scores for marginal gap were
68 µm for chamfer and 63 µm for shoulder margin
con-figurations; which were close to the results of similar
previous studies. Hertlain et al.  explored the
mar-ginal fit of Lava CAD/CAM all-ceramic system with a
chamfer preparation and reported the marginal
adapta-tion to vary between 40-70 µm. Tao et al.  reported
that the marginal gap of Cercon crowns ranged from 40
to 90 µm. Mirza Rustam Baig et al.  also examined
marginal fit of Cercon zirconia crowns and suggested
the overall mean marginal gap of 66.4 µm. Moreover,
they reported that margin configuration did not
signifi-cantly affect the marginal gap of complete coverage
Cercon crowns.Still in another study, Bindl and
Mor-mann  compared the marginal discrepancy using
Cercon zirconia material with chamfer and shoulder
finish lines and reported comparable results regarding
both finish lines.
In a compelling study, Kyu-Bok Lee et al. 
evaluated the marginal fit of conventional double
lay-ered CAD/CAM system (Porcera) on metal dies with 1
mm shoulder margin. They found that after the
porce-lain firing, the marginal discrepancy width of Porcera
crowns (89.6±9.5 µm) demonstrated significantly larger
gaps than that of Porcera copings (72.2±7.0 µm) (p<
0.05). This difference, which was also observed in our
study, could be justified by the fact that the porcelain
veneering procedure makes the particles of porcelains
melt and gather to fill up the gaps. Therefore, the
result-ing contraction of porcelain mass imposes a
compres-sive force on the coping.  The consequent
defor-mation of coping spreads over the whole circumference
of the margin under the pressure of contracting
porce-lain.  Nevertheless, it must be noted that the
mar-ginal openings of the crowns after the porcelain
veneer-ing are within clinically acceptable standards, and the
amount of deformation does not interfere with the
Considering the layered restorations, a positive
thermal mismatch will always lead to formation of
ten-sile stress within the framework. While the veneering
ceramic is subjected to compressive forces, a negative
mismatch will produce a completely reverse effect. We
are well aware that dental manufacturers have come
along all-ceramic systems which appear to have
veneer-ing ceramics of slightly lower coefficient of thermal
expansion (CTEs) than that of the framework, resulting
in a positive mismatch of the CTEs. This positive
mis-match is expected to induce a beneficial compression
stress on the veneering porcelain layer.  Aboushelib
et al. presumed that minimizing the thermal
mis-match would be desirable, especially for all-ceramic
zirconia restorations. However, Isgro et al. declared
that even a zero thermal mismatch value is not enough
to predict compatibility between ceramic core and
ve-neering porcelain. According to these reports, there are
other factors that need to be considered, including
vis-coelastic behavior of the porcelain, repeated firings, and
fast or slow cooling procedures.
It can be concluded from the outcome of the
aforementioned studies that the distortion of marginal fit
could be due to the shrinkage of porcelain as a result of
coping distortion, CTE incompatibility of the core and
the veneering porcelain, and porcelain contamination of
the internal surface of the copings.
As mentioned previously, porcelain firing cycles
change the marginal fit of shoulder copings more
ad-versely compared with rounded chamfer copings. The
the chamfer finish line has some length on axial wall of
the preparation, so the closing of margin i more
proba-ble along this length. On the other hand, shoulder
mar-gin has a butt joint form, without any length on axial
wall. This is why if any distortion happens due to
porce-lain firing, it will affect the whole marginal gap. In
agreement with the current study, Pera et al.  that
evaluated the marginal adaptation of porcelain ceramic
crowns reported improved marginal fit of In-Ceram
crowns fabricated on chamfer compared with shoulder
finish line, although they did not explain the cause.
Certainly, this study was not free of limitations.
Some of these restrictions are discussed as follows.
First, marginal fit was measured in this experimental
design; however, the internal fit of the crowns was not.
The reason was that measuring the internal fit of the
crowns required the crowns to be cemented and the
specimens to be sectioned. Second, all copings were
produced and tested under ideal conditions, which may
not reflect the conditions which can be seen in daily
clinical practices. Third, the copings were not subjected
to mechanical and thermal cycling; while thermo
me-chanical cycling is one of the most important factors
which affects the long-term success of the restoration.
[41-42] Finally, although brass dies were used for
measurement, use of human natural teeth would be
Within the limitations of this study, the following
con-clusions could be drawn:
1. Porcelain veneering showed to have a statistically
significant influence on the marginal fit of zirconia
2. There were no significant differences between
completed crowns of chamfer and shoulder
3. Both margin configurations demonstrated marginal
gaps that were within a reported clinically
accepta-ble range of marginal discrepancy.
The authors thank the Vice-Chancellery of Shiraz
Uni-versity of Medical Sciences for supporting this research
study (Grant#91-01-03-4689). The article was based on
a thesis by Dr. Mina Mohaghegh. The authors also
thank Dr. Salehi from the Dental Research
Develop-ment Center, School of Dentistry for his contributions in
the process of statistical analyses.
Conflict of Interest No conflict of interest.
 Rosensteil SF, Land MF, Fujimoto J. Contemporary fixed prosthodontics. 4th ed. St.Louis: Elsevier; 2006. p. 774.
 Jones DW. Development of dental ceramics. An histor-ical perspective. Dent Clin North Am 1985; 29: 621-644.
 Schneider W. Cerec 3. Int J Comput Dent 2000; 3: 33-40.
 Kohorst P, Brinkmann H, Dittmer MP, Borchers L, Stiesch M. Influence of the veneering process on the marginal fit of zirconia fixed dental prostheses. J Oral Rehabil 2010; 37: 283-291.
 Raigrodski AJ. Contemporary materials and technolo-gies for all-ceramic fixed partial dentures: a review of the lite rature. J Prosthet Dent 2004; 92: 557-562.  Oilo M, Gjerdet NR, Tvinnereim HM. The firing
pro-cedure influences properties of a zirconia core ceramic. Dent Mater 2008; 24: 471-475.
 Karlsson S. The fit of Procera titanium crowns. An in vitro and clinical study. Acta Odontol Scand 1993; 51: 129-134.
 Odén A, Andersson M, Krystek-Ondracek I, Magnus-son D. Five-year clinical evaluation of Procera AllCe-ram crowns. J Prosthet Dent 1998; 80: 450-456.  Sailer I, Fehér A, Filser F, Gauckler LJ, Lüthy H,
Hämmerle CH. Five-year clinical results of zirconia frameworks for posterior fixed partial dentures. Int J Prosthodont 2007; 20: 383-388.
Sailer I, Pjetursson BE, Zwahlen M, Hämmerle CH. A systematic review of the survival and complication rates of all-ceramic and metal-ceramic reconstructions after an observation period of at least 3 years. Part II: Fixed dental prostheses. Clin Oral Implants Res 2007; 18 Suppl 3: 86-96.
Jacobs MS, Windeler AS. An investigation of dental luting cement solubility as a function of the marginal gap. J Prosthet Dent 1991; 65: 436-442.
partial dentures. J Prosthet Dent 2000; 84: 492-498. Della Bona A, Kelly JR. The clinical success of
all-ceramic restorations. J Am Dent Assoc 2008; 139 Suppl : 8S-13S.
Felton DA, Kanoy BE, Bayne SC, Wirthman GP. Effect of in vivo crown margin discrepancies on periodontal health. J Prosthet Dent 1991; 65: 357-364.
Balkaya MC, Cinar A, Pamuk S. Influence of firing cycles on the margin distortion of 3 all-ceramic crown systems. J Prosthet Dent 2005; 93: 346-355.
Holmes JR, Sulik WD, Holland GA, Bayne SC. Mar-ginal fit of castable ceramic crowns. J Prosthet Dent 1992; 67: 594-599.
Holmes JR, Bayne SC, Holland GA, Sulik WD. Con-siderations in measurement of marginal fit. J Prosthet Dent 1989; 62: 405-408.
McLean JW, von Fraunhofer JA. The estimation of cement film thickness by an in vivo technique. Br Dent J 1971; 131: 107-111.
Pera P, Gilodi S, Bassi F, Carossa S. In vitro marginal adaptation of alumina porcelain ceramic crowns. J Prosthet Dent 1994; 72: 585-590.
Shearer B, Gough MB, Setchell DJ. Influence of mar-ginal configuration and porcelain addition on the fit of In-Ceram crowns. Biomaterials 1996; 17: 1891-1895. Coli P, Karlsson S. Fit of a new pressure-sintered
zirco-nium dioxide coping. Int J Prosthodont 2004; 17: 59-64. Tinschert J, Natt G, Mautsch W, Spiekermann H, Anusavice KJ. Marginal fit of alumina-and zirconia-based fixed partial dentures produced by a CAD/CAM system. Oper Dent 2001; 26: 367-374.
Tao J, Han D. The effect of finish line curvature on marginal fit of all-ceramic CAD/CAM crowns and met-al-ceramic crowns. Quintessence Int 2009; 40: 745-752. Baig MR, Tan KB, Nicholls JI. Evaluation of the
mar-ginal fit of a zirconia ceramic computer-aided machined (CAM) crown system. J Prosthet Dent 2010; 104: 216-227.
Chevalier J. What future for zirconia as a biomaterial? Biomaterials 2006; 27: 535-543.
Castellani D, Baccetti T, Clauser C, Bernardini UD. Thermal distortion of different materials in crown con-struction. J Prosthet Dent 1994; 72: 360-366.
Pak HS, Han JS, Lee JB, Kim SH, Yang JH. Influence of porcelain veneering on the marginal fit of Digident and Lava CAD/CAM zirconia ceramic crowns. J Adv
Prosthodont 2010; 2: 33-38.
Goodacre CJ, Campagni WV, Aquilino SA. Tooth preparations for complete crowns: an art form based on scientific principles. J Prosthet Dent 2001; 85: 363-376. Suárez MJ, González de Villaumbrosia P, Pradíes G, Lozano JF. Comparison of the marginal fit of Procera AllCeram crowns with two finish lines. Int J Prostho-dont 2003; 16: 229-232.
Comlekoglu M, Dundar M, Ozcan M, Gungor M, Gokce B, Artunc C. Influence of cervical finish line type on the marginal adaptation of zirconia ceramic crowns. Oper Dent 2009; 34: 586-592.
Quintas AF, Oliveira F, Bottino MA. Vertical marginal discrepancy of ceramic copings with different ceramic materials, finish lines, and luting agents: an in vitro evaluation. J Prosthet Dent 2004; 92: 250-257. Akbar JH, Petrie CS, Walker MP, Williams K, Eick JD.
Marginal adaptation of Cerec 3 CAD/CAM composite crowns using two different finish line preparation de-signs. J Prosthodont 2006; 15: 155-163.
Sorensen JA. A standardized method for determination of crown margin fidelity. J Prosthet Dent 1990; 64: 18-24.
Komine F, Iwai T, Kobayashi K, Matsumura H. Mar-ginal and internal adaptation of zirconium dioxide ce-ramic copings and crowns with different finish line de-signs. Dent Mater J 2007; 26: 659-664.
Hertlein G, Hoscheler S, Frank S, Suttor D. Marginal fit of CAD/CAM manufactured all ceramic prosthesis. J Dent Res 2001; 80: 42-44.
Bindl A, Mörmann WH. Fit of all-ceramic posterior fixed partial denture frameworks in vitro. Int J Perio-dontics Restorative Dent 2007; 27: 567-575.
Lee KB, Park CW, Kim KH, Kwon TY. Marginal and internal fit of all-ceramic crowns fabricated with two different CAD/CAM systems. Dent Mater J 2008; 27: 422-426.
Weaver JD, Johnson GH, Bales DJ. Marginal adapta-tion of castable ceramic crowns. J Prosthet Dent 1991; 66: 747-753.
Aboushelib MN, Matinlinna JP, Salameh Z, Ounsi H. Innovations in bonding to zirconia-based materials: Part I. Dent Mater 2008; 24: 1268-1272.
ter 2005; 21: 649-655.
Vojdani M, Torabi K, Farjood E, Khaledi A. Compari-son the Marginal and Internal Fit of Metal Copings Cast from Wax Patterns Fabricated by CAD/CAM and Con-ventional Wax up Techniques. J Dent (Shiraz) 2013; 14: 118-129.